Available online at www.sciencedirect.com
Solid-State Electronics 52 (2008) 844–848 www.elsevier.com/locate/sse
Channel width dependence of hot electron injection program/hot hole erase cycling behavior in silicon-oxide-nitride-oxide-silicon (SONOS) memories Seung-Hwan Seo a, Se-Woon Kim a, Jang-Uk Lee a, Gu-Cheol Kang a, Kang-Seob Roh a, Kwan-Young Kim a, Soon-Young Lee a, Chang-Min Choi a, Kwan-Jae Song a, So-Ra Park a, Jun-Hyun Park a, Ki-Chan Jeon a, Dong Myong Kim a, Dae Hwan Kim a,*, Hyungcheol Shin b, Jong Duk Lee b, Byung-Gook Park b a
School of Electrical Engineering, Kookmin University, 861-1, Jeongnung-dong, Seongbuk-gu, Seoul 136-702, Republic of Korea School of Electrical Engineering, Seoul National University, San 56-1, Shinlim-dong, Kwanak-gu, Seoul 151-742, Republic of Korea Received 10 August 2007; received in revised form 27 November 2007; accepted 4 February 2008 Available online 7 March 2008
The review of this paper was arranged by Prof. S. Cristoloveanu
Abstract The channel width dependence of hot electron injection program/hot hole erase cycling behavior in silicon-oxide-nitride-oxide-silicon (SONOS) memories is investigated. While the trapped charge proﬁle-dependent overerasure is observed in 10-lm-wide device, it is suppressed in 0.22-lm-wide device. Both the overerasure suppression and gradual positive threshold voltage shift in narrow device are explained as an elevated hot hole injection eﬃciency followed by more pronounced redistribution of the hole proﬁle in the channel-center and the suppression of the lateral migration of injected holes in the channel-edge, by combining the measured endurance characteristics and TCAD simulation results. Main physical mechanisms are three-dimensional distribution of the electric ﬁeld by gate/drain voltage, increasing interface states, and their trapped charge with cycling in the channel-edge. Ó 2008 Elsevier Ltd. All rights reserved. Keywords: Silicon-oxide-nitride-oxide-silicon; SONOS; Hot electron injection program; Hot hole erase; Width dependence; Cycling behavior
1. Introduction The nonvolatile silicon-oxide-nitride-oxide-silicon (SONOS) memories have been recently attracted much attention as emerging candidates for next generation ﬂash memories in terms of a simple manufacturing process, small cell size, low voltage operation, endurance to extended program/erase (P/E) cycling, and no drain turnon . Especially, for the purpose of multi-bit operation per cell, their NROM (nitride read only memory)-type P/E scheme has been widely used , which is based on a *
Corresponding author. Tel.: +82 2 910 4872; fax: +82 2 910 4449. E-mail address: [email protected]
n.ac.kr (D.H. Kim).
0038-1101/$ - see front matter Ó 2008 Elsevier Ltd. All rights reserved. doi:10.1016/j.sse.2008.02.001
channel hot electron injection (CHEI) program/a hot hole injection (HHI) erase, respectively. In the case of NROMtype SONOS memories, the overerasure is a challenging issue to overcome, because it makes a threshold voltage (VT) window uncontrollable. The overerasure mechanism has been explained as accumulated positive charges above source/drain n+ junction, drain-induced barrier lowering (DIBL) in short channel devices, and the lateral migration of trapped charges in nitride storage layer after P/E cycles [3–6]. While various works on their reliability and scaling eﬀect with the channel length (L) have been actively reported [3,4], the channel width (W) dependence of SONOS devices has been rarely studied in comparison with its importance.
S.-H. Seo et al. / Solid-State Electronics 52 (2008) 844–848
In this work, we report the channel width eﬀect of P/E cycling behavior in SONOS memory devices. The experiment is focused on endurance characteristic and combined with SENTAURUS TCAD simulation. It is shown that the W-dependence of endurance characteristics in NROM-type SONOS devices is strongly related with the diﬀerence of both the lateral electric ﬁeld-dependent HHI eﬃciency and the proﬁle of accumulated holes between a channelcenter and channel-edge. 2. Experimental results In order to investigate the W-dependence of P/E cycling behavior, SONOS devices with diﬀerent channel widths and the same channel length (W/L = 0.22/0.24 and 10/ 0.24 lm) were characterized. They were fabricated on the 4 1015 cm 3 boron-doped p-type silicon substrate using a conventional 0.18 lm CMOS process technology. Conventional channel implantation was performed for VT adjustment, and additional pocket implantation was not used. In order to consider the narrow with eﬀect in MOSFET, the shallow trench isolation (STI) technique was used for the device isolation. Thickness of each layer in the oxide-nitride-oxide (ONO) stack was 4 nm (top oxide), 4 nm (nitride) and 4 nm (bottom oxide), respectively. VT was deﬁned as the applied gate voltage VG where the drain current (ID) at the drain voltage VD = 0.1 V is 0.1 lA in narrow device and 10 lA in wide device, respectively. Endurance tests were done to up to 10,000 cycles. P/E and read conditions are speciﬁed in Table 1. There are two diﬀerent P/E conditions from typical NROM-type: the negative substrate bias in erase operation (VB = 4 V) and the small drain bias in reverse read operation (VD = 0.1 V). The former is due to the test device situation that the negative VGB is not allowed because the electrostatic discharge (ESD) protection diode is integrated with test pattern between gate and substrate contacts. Negative VB makes the depletion region between the drain and substrate such wider that a HHI erase becomes more eﬃcient at the same VGD. The latter is intended in order to suppress DIBL eﬀect because we focus only the W-dependence. Although a high read voltage (VD) is favorable to control the second bit eﬀect in NROM-type reverse read scheme , the typical DIBL in short channel devices should be excluded for characterizing the W-dependence. Therefore, used P/E and read conditions are thought not to lose the validity of characterizing the W-dependent endurance in NROM devices.
Fig. 1 shows the current–voltage (I–V) characteristics with P/E cycling. The P/E cycling behavior of NROM erased cell has been investigated in many literatures and commonly accepted to be caused by the P/E cycling-evolution of the lateral charge proﬁle along the channel length direction in nitride storage layer. Shappir et al. investigated the P/E condition-dependence of the drift of an erased VT (VTE) (as the function of a time) and explained that the dipole-induced electric ﬁeld due to the misalignment between the distributions of the injected electrons and injected holes led to the lateral migration of the holes followed by the VTE drift. In addition, the VTE drift became alleviated with P/E cycles due to the accumulated holes above the source junction [3,5]. On the other hand, according to Furnemont et al., the degradation of both the VT window and the subthreshold slope with P/E cycles is mainly caused by the cycling-evolution of the nitride charge proﬁle resulting from the lateral location mismatch of electrons and holes even in the case of the degraded devices in terms of the interface states [6,8]. We note that these previous works have been focused on the redistribution of nitride charge not along the channel width direction but along the channel length direction. Fig. 2 shows the W-dependence of P/E cycling behavior at various erase conditions (VD = 3.5, 4, 4.5 V, respectively). In the case of 10-lm-wide device, while the negative shift followed by saturation of VTE is observed, the programmed VT (VTP) is hardly shifted with P/E cycling, as shown in Fig. 2a. Moreover, VTE is very sensitive to VD values in various erase operations under the same program
Table 1 Program/Erase and read conditions of the measured SONOS memories Operation condition
Program Erase Reverse read
5.5 3.5–4.5 0
5.5 4 Sweep
0 0 0.1
25 ls 1 ms
TP and TE represent the program and erase pulse times, respectively.
Fig. 1. The current–voltage characteristics after P/E cycles of (a) 10-lmwide device and (b) 0.22-lm-wide device, respectively.
S.-H. Seo et al. / Solid-State Electronics 52 (2008) 844–848
Fig. 2. The width dependence of the P/E cycling behavior at VD values in various erase operation conditions of (a) 10-lm-wide device and (b) 0.22lm-wide device, respectively.
condition. It shows that the P/E cycling behavior of VTE is related to the HHI eﬃciency, because the lateral electric ﬁeld (ELAT) is proportional to HHI eﬃciency. The overerasure in 10-lm-wide device becomes more pronounced as the value of VD in the HHI erase operation increases. It can be explained by more pronounced redistribution of the hole proﬁle along the channel length direction in nitride layer resulting from increasing amount of the accumulated excess holes with the P/E cycles. Moreover, the hole is more widely distributed with increasing P/E cycles as VD increases in an erase operation . Fig. 2a shows that the overerasure cannot be controlled by lowering VD in HHI erase operation because of a trade-oﬀ with VT window margin. Previous studies show that the optimized CHEI program condition is critical to suppress the overerasure inas much as the migration of lateral proﬁle of trapped charge, i.e., the spatial mismatch of injected electrons and holes, is the root cause of retention degradation of NROM devices [6,8]. The VTE at VD = 4.5 V is saturated as the number of P/E cycles increases because of the self-limited erase eﬃciency. Therefore, the endurance characteristic of 10-lm-wide device is consistent with the previously reported mechanisms. However, in the case of 0.22-lm-wide device, no overerasure is observed as shown in Fig. 2b. On the contrary, both VTE and VTP show a gradual positive shift with P/E cycles. This should be explained by combining the W-eﬀect with the overerasure mechanism in wide devices. In terms of the W-eﬀect, the STI-induced stress in the channel-edge region is known to induce the reliability degradation as VT
shift, additional interface trap generation, and gm reduction in narrow MOSFETs [10,11]. However, in our case, the degradation of subthreshold slope as the sign of interface traps increasing with P/E cycles is not observed in erased cell as shown in Fig. 1. It means that the interface states formed in the local HHI region will not be sensed by the subthreshold slope in the erased cell because the local VTE will be the lowest there whereas they can be sensed by the subthreshold slope of the programmed cell. On the other hand, the degraded subthreshold slope in NROM programmed cell is also the sign not only of the interface states but also of locally trapped electrons at the nitride layer that causes the fringing ﬁeld eﬀect in the channel surface region . Therefore, it should be addressed whether the observed W-dependence is originated from the cycle-evolution of the interface states or that of the distribution of nitride charge. Fig. 3 shows the cycle-evolution of the ﬂat band voltage VFB which is extracted by measuring the gated-diode current in another diﬀerent devices from those in Fig. 2 (VD = 4 V at the erase condition). The cycle-dependences of the VFB’s in both the 10-lm-wide device and the 0.22-lm-wide device are the same with those of VTE’s. It shows that the W-dependence of P/E cycling behavior is mainly caused by the cycle-evolution of the distribution of nitride charge rather than that of the interface states. It is consistent with the previously reported work that the subthreshold slope of NROM device is determined by the proﬁle of locally trapped charge rather than interface trap density [8,12,13]. However, paradoxically, it should be noticed that the interface trap can increase during P/E cycles without the degradation of subthreshold slope of the erased cell in the case of NROM device.
Fig. 3. The P/E cycling behaviors of both VT and VFB in (a) 0.22-lm-wide device and (b) 10-lm-wide device, respectively.
S.-H. Seo et al. / Solid-State Electronics 52 (2008) 844–848
Fig. 4. The simulation result of the lateral electric ﬁeld (ELAT) distribution in channel-center and channel-edge region at a depth of 50 nm from the Si/ bottom oxide interface under erase condition at VD/VG/VS/VB = 4/ 4/0/ 4 V. (a) 10-lm-wide device and (b) 0.22-lm-wide device, respectively. The inset shows the schematic diagram of the 3D distribution of the electric ﬁeld by VD/VG.
In order to verify the W-dependence, three-dimensional (3D) TCAD simulation is conducted using the SENTAURUS TCAD simulator. Fig. 4 shows the simulated ELAT at a depth of 50 nm from the Si/bottom oxide interface. The amplitude of ELAT in channel-center is larger than that in channel-edge, commonly in wide and narrow device. Furthermore, the diﬀerence between in channel-center and channel-edge region becomes larger in 0.22-lm-wide device than in 10-lm-wide device. It is originated from the diﬀerence in the channel controllability of VG/VD between the channel-center and edge region, as shown in the inset of Fig. 4. Our result shows that eﬀectively higher VD results in higher HHI eﬃciency in the center region, which means that more holes are injected and widely distributed along the channel length direction in the center region than in the edge region after an erase operation . Fig. 5 shows the schematic VT distribution explaining W-dependent endurance mechanism. As the lateral proﬁle of injected holes becomes more widely distributed, the excess holes redistributed along the channel length direction are less compensated by the electrons injected in the next program operation. In other word, more severe spatial mismatch between injected electrons and holes increases accumulated holes during P/E cycling in the channel-center rather than the channel-edge. Consequently, the eﬀect of a lower local VTE in the center than the edge becomes more
Fig. 5. Schematic VT distribution after P/E cycling in (a) the channel-center region and (b) the channel-edge region.
S.-H. Seo et al. / Solid-State Electronics 52 (2008) 844–848
dominant in 10-lm-wide device, which induces an overerasure shown in Fig. 2a. As W becomes narrower, the eﬀect of a higher local VTE in the edge than in the center becomes more dominant. This is the mechanism of suppressed overerasure in 0.22-lm-wide device. Moreover, slight increase of both VTP and VTE with P/E cycles in 0.22-lm-wide device (Fig. 2b) is well explained by a higher channel-edge VT due to both the increasing interface states and their trapped electrons as the number of P/E cycles increases. This mechanism is not inconsistent with the subthreshold slope in erased cell as mentioned above. Furthermore, the vertical electric ﬁeld (EVER) larger in the channel-edge than the channel-center accelerates the generation of interface states in the channel-edge region during the program operation. It results in increasing trapped electrons followed by an additional hole-attractive EVER in the channeledge region during the erase operation. Therefore, the redistribution of the hole proﬁle is such retarded in the channel-edge region that both the suppressed overerasure and positive shift of VT with P/E cycles becomes more strengthened. 4. Conclusions The W-dependence of P/E cycling behavior in NROMtype SONOS memories was investigated. Both the overerasure suppression and gradual positive VT shift in narrow device were explained as an elevated HHI eﬃciency in the channel-center region and a suppression of the redistribution of holes injected in the channel-edge region, by combining the measured endurance characteristics and 3D TCAD simulation results. Main physical mechanisms are more pronounced redistribution of the hole proﬁle in the channel-center due to the 3D distribution of the electric ﬁeld by VG/VD, the interface states, and their trapped charge increasing with P/E cycling in the channel-edge region. Our results provide a physical insight on the Wdependence of P/E cycling behavior in SONOS memories. Acknowledgement This work was supported by of Kookmin University (Korea) under Research Program, and the CAD software was supported by the IC Design Education Center (IDEC).
References  Bu J, White MH. Design considerations in scaled SONOS nonvolatile memory devices. Solid-State Electr ICS 2001;45:113–20.  Eitan B, Pavan P, Bloom I, Aloni E, Frommer A, Finzi D. NROM: A novel localized trapping, 2-bit nonvolatile memory cell. IEEE Electr Dev Lett 2000;21:543–5.  Shappir A, Shacham-Diamond Y, Lusky E, Bloom I, Eitan B. Lateral charge transport in the nitride layer of the NROM nonvolatile memory device. Microelect Eng 2004;72:426–33.  Yeh CC, Wang T, Tsai WJ, Lu TC, Liao YY, Chen HY, et al. A novel erase scheme to suppress overerasure in a scaled 2-bit nitride storage ﬂash memory cell. IEEE Electr Dev Lett 2004;25:643–5.  Shappir A, Levy D, Shacham-Diamond Y, Lusky E, Bloom I, Eitan B. Spatial characterization of localized charge trapping and charge redistribution in the NROM device. Solid-State Electr 2004;48: 1489–95.  Furnemont A, Rosmeulen M, Van Houdt J, Maes H, De Meyer K. Cycling behavior of nitride charge proﬁle in NROM-type memory cells. Proc. IEEE Non-Volatile Semiconductor Memory Workshop 2006:66–7.  Lue HT, Hsu TH, Wu MT, Hsieh KY, Liu R, Lu CY. Studies of the reverse read method and second-bit eﬀect of 2-bit/cell nitridetrapping device by quasi-two-dimensional model. IEEE Trans Electr Dev 2005;53:119–25.  Furnemont A, Rosmeulen M, Van der Zanden K, Van Houdt J, De Meyer K, Maes H. Root cause of charge loss in a nitride-based localized trapping memory cell. IEEE Trans Electr Dev 2007;54: 1351–9.  Furnemont A, Rosmeulen M, Van der Zanden K, Van Houdt J, De Meyer K, Maes H. New operating mode based on electron/hole proﬁle matching in nitride-based nonvolatile memories. IEEE Electr Dev Lett 2007;28:276–8.  Nishigohri M, Ishimaru K, Takahashi M, Unno Y, Okayama Y, Matsuoka F, et al. Anomalous hot-carrier induced degradation in very narrow channel nMOSFET’s with STI structure. Tech Dig Int Electr Dev Meet 1996:881–4.  Lee JD, Choi JH, Park D, Kim K. Eﬀects of interface trap generation and annihilation on the data retention characteristics of ﬂash memory cells. IEEE Trans Device Mater Reliab 2004;4:110–7.  Shappir A, Shacham-Diamond Y, Lusky E, Bloom I, Eitan B. Subthreshold slope degradation model for localized-charge-trapping based non-volatile memory devices. Solid-State Electr 2003;47: 937–41.  Lusky E, Shacham-Diamond Y, Bloom I, Eitan B. Characterization of channel hot electron injection by the subthreshold slope of NROM device. IEEE Electr Dev Lett 2001;22:556–8.